#------------------------------------------------------------------------------
#$Date: 2016-02-16 03:10:39 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176453 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/48/7204806.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7204806
loop_
_publ_author_name
'Laura León-Reina'
'Enrique R. Losilla'
'María Martínez-Lara'
'Sebastián Bruque'
'Miguel A. G. Aranda'
_publ_section_title
;
 Interstitial oxygen conduction in lanthanum oxy-apatite electrolytes
;
_journal_issue                   7
_journal_name_full               'J. Mater. Chem.'
_journal_page_first              1142
_journal_page_last               1149
_journal_paper_doi               10.1039/b315257j
_journal_volume                  14
_journal_year                    2004
_chemical_formula_sum            'Ge La1.6 O4.43'
_chemical_formula_weight         365.70
_chemical_name_systematic        ' ?'
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_audit_creation_date             2003-09-18T17:07
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
;
2003-09-18T17:07  Initial CIF as created by GSAS2CIF
;
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            6
_cell_length_a                   9.96580(19)
_cell_length_b                   9.9658
_cell_length_c                   7.31160(16)
_cell_volume                     628.879(18)
_computing_structure_refinement  GSAS
_pd_block_id
2003-09-18T17:07|La960Ge_773k|La960Ge_773K|Overall
_pd_phase_name
'from C:/users/leon/La960GeGe_sinQ/La960Ge(O4).EXP'
_refine_ls_goodness_of_fit_all   2.09
_refine_ls_matrix_type           full
_refine_ls_number_parameters     72
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.38
_refine_ls_shift/su_mean         0.08
_cod_data_source_file            b315257j.txt
_cod_data_source_block           La960Ge_773k_publ
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (152
times).

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (63 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        628.87958
_cod_original_formula_sum        'Ge La1.60 O4.43'
_cod_database_code               7204806
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 x-y,+x,+z+1/2
3 -y,x-y,+z
4 -x,-y,+z+1/2
5 y-x,-x,+z
6 +y,y-x,+z+1/2
-1 -x,-y,-z
-2 y-x,-x,-z+1/2
-3 +y,y-x,-z
-4 +x,+y,-z+1/2
-5 x-y,+x,-z
-6 -y,x-y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
LA La1 0.22897(22) -0.01249(27) 0.25 1.0 Uani 0.02777 6
LA La2 0.3333 0.6667 0.0034(4) 0.9 Uani 0.03354 4
GE Ge 0.40015(24) 0.37321(22) 0.25 1.0 Uani 0.02234 6
O O1 0.3132(4) 0.4869(4) 0.25 1.0 Uani 0.05092 6
O O2 0.60202(34) 0.47181(34) 0.25 1.0 Uani 0.03934 6
O O3 0.3428(4) 0.24979(29) 0.06095(29) 1.0 Uani 0.06446 12
O O4 0.0 0.0 0.25 0.937(13) Uani 0.06959 2
O O5 0.010(5) 0.234(5) 0.605(4) 0.058(4) Uiso 0.03 12
loop_
_atom_type_symbol
_atom_type_number_in_cell
LA 9.6
GE 6.0
O 26.57
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 La1 O2 98.42(12) 5_555 . 3_655 n
O1 La1 O3 145.32(7) 5_555 . 1_555 n
O1 La1 O3 69.45(9) 5_555 . 6_555 n
O1 La1 O3 69.45(9) 5_555 . -3_555 n
O1 La1 O3 145.32(7) 5_555 . -4_556 n
O1 La1 O4 112.68(11) 5_555 . 1_555 n
O1 La1 O5 57.5(8) 5_555 . 4_554 n
O1 La1 O5 91.0(10) 5_555 . 5_555 n
O1 La1 O5 154.1(6) 5_555 . 6_554 n
O1 La1 O5 57.5(8) 5_555 . -1_556 n
O1 La1 O5 91.0(10) 5_555 . -2_556 n
O1 La1 O5 154.1(6) 5_555 . -3_556 n
O2 La1 O3 69.58(11) 3_655 . 1_555 n
O2 La1 O3 85.24(8) 3_655 . 6_555 n
O2 La1 O3 85.24(8) 3_655 . -3_555 n
O2 La1 O3 69.58(11) 3_655 . -4_556 n
O2 La1 O4 148.89(14) 3_655 . 1_555 n
O2 La1 O5 143.5(8) 3_655 . 4_554 n
O2 La1 O5 90.9(8) 3_655 . 5_555 n
O2 La1 O5 90.5(9) 3_655 . 6_554 n
O2 La1 O5 143.5(8) 3_655 . -1_556 n
O2 La1 O5 90.9(8) 3_655 . -2_556 n
O2 La1 O5 90.5(9) 3_655 . -3_556 n
O3 La1 O3 137.65(12) 1_555 . 6_555 n
O3 La1 O3 77.02(6) 1_555 . -3_555 n
O3 La1 O3 62.67(11) 1_555 . -4_556 n
O3 La1 O4 84.03(10) 1_555 . 1_555 n
O3 La1 O5 113.1(7) 1_555 . 4_554 n
O3 La1 O5 120.7(10) 1_555 . 5_555 n
O3 La1 O5 22.8(9) 1_555 . 6_554 n
O3 La1 O5 145.9(8) 1_555 . -1_556 n
O3 La1 O5 58.0(10) 1_555 . -2_556 n
O3 La1 O5 60.5(6) 1_555 . -3_556 n
O3 La1 O3 135.78(20) 6_555 . -3_555 n
O3 La1 O3 77.02(6) 6_555 . -4_556 n
O3 La1 O4 105.12(9) 6_555 . 1_555 n
O3 La1 O5 107.4(8) 6_555 . 4_554 n
O3 La1 O5 23.5(10) 6_555 . 5_555 n
O3 La1 O5 135.8(7) 6_555 . 6_554 n
O3 La1 O5 61.5(8) 6_555 . -1_556 n
O3 La1 O5 159.2(11) 6_555 . -2_556 n
O3 La1 O5 87.3(6) 6_555 . -3_556 n
O3 La1 O3 137.65(12) -3_555 . -4_556 n
O3 La1 O4 105.12(9) -3_555 . 1_555 n
O3 La1 O5 61.5(8) -3_555 . 4_554 n
O3 La1 O5 159.2(11) -3_555 . 5_555 n
O3 La1 O5 87.3(6) -3_555 . 6_554 n
O3 La1 O5 107.4(8) -3_555 . -1_556 n
O3 La1 O5 23.5(10) -3_555 . -2_556 n
O3 La1 O5 135.8(7) -3_555 . -3_556 n
O3 La1 O4 84.03(10) -4_556 . 1_555 n
O3 La1 O5 145.9(8) -4_556 . 4_554 n
O3 La1 O5 58.0(10) -4_556 . 5_555 n
O3 La1 O5 60.5(6) -4_556 . 6_554 n
O3 La1 O5 113.1(7) -4_556 . -1_556 n
O3 La1 O5 120.7(10) -4_556 . -2_556 n
O3 La1 O5 22.8(9) -4_556 . -3_556 n
O4 La1 O5 62.0(8) 1_555 . 4_554 n
O4 La1 O5 88.6(8) 1_555 . 5_555 n
O4 La1 O5 61.5(10) 1_555 . 6_554 n
O4 La1 O5 62.0(8) 1_555 . -1_556 n
O4 La1 O5 88.6(8) 1_555 . -2_556 n
O4 La1 O5 61.5(10) 1_555 . -3_556 n
O5 La1 O5 114.4(14) 4_554 . 5_555 n
O5 La1 O5 101.9(15) 4_554 . 6_554 n
O5 La1 O5 49.5(15) 4_554 . -1_556 n
O5 La1 O5 65.0(9) 4_554 . -2_556 n
O5 La1 O5 123.5(14) 4_554 . -3_556 n
O5 La1 O5 113.2(14) 5_555 . 6_554 n
O5 La1 O5 65.0(9) 5_555 . -1_556 n
O5 La1 O5 177.0(18) 5_555 . -2_556 n
O5 La1 O5 64.5(10) 5_555 . -3_556 n
O5 La1 O5 123.5(14) 6_554 . -1_556 n
O5 La1 O5 64.5(10) 6_554 . -2_556 n
O5 La1 O5 48.7(13) 6_554 . -3_556 n
O5 La1 O5 114.4(14) -1_556 . -2_556 n
O5 La1 O5 101.9(15) -1_556 . -3_556 n
O5 La1 O5 113.2(14) -2_556 . -3_556 n
La2 La2 La2 179.9604 -2_565 . -2_566 n
La2 La2 O1 136.67(7) -2_565 . 1_555 n
La2 La2 O1 136.67(7) -2_565 . 3_665 n
La2 La2 O1 136.71(7) -2_565 . 5_565 n
La2 La2 O2 44.05(7) -2_565 . 2_554 n
La2 La2 O2 44.04(7) -2_565 . 4_664 n
La2 La2 O2 44.03(7) -2_565 . 6_564 n
La2 La2 O1 43.32(7) -2_566 . 1_555 n
La2 La2 O1 43.31(7) -2_566 . 3_665 n
La2 La2 O1 43.32(7) -2_566 . 5_565 n
La2 La2 O2 135.98(7) -2_566 . 2_554 n
La2 La2 O2 135.94(7) -2_566 . 4_664 n
La2 La2 O2 135.96(7) -2_566 . 6_564 n
O1 La2 O1 72.89(11) 1_555 . 3_665 n
O1 La2 O1 72.90(11) 1_555 . 5_565 n
O1 La2 O2 124.95(9) 1_555 . 2_554 n
O1 La2 O2 95.00(7) 1_555 . 4_664 n
O1 La2 O2 155.33(10) 1_555 . 6_564 n
O1 La2 O1 72.90(11) 3_665 . 5_565 n
O1 La2 O2 155.37(10) 3_665 . 2_554 n
O1 La2 O2 124.93(9) 3_665 . 4_664 n
O1 La2 O2 95.02(7) 3_665 . 6_564 n
O1 La2 O2 95.03(7) 5_565 . 2_554 n
O1 La2 O2 155.35(10) 5_565 . 4_664 n
O1 La2 O2 124.97(9) 5_565 . 6_564 n
O2 La2 O2 74.03(11) 2_554 . 4_664 n
O2 La2 O2 74.03(11) 2_554 . 6_564 n
O2 La2 O2 74.02(11) 4_664 . 6_564 n
O1 Ge O2 116.36(21) 1_555 . 1_555 n
O1 Ge O3 111.42(13) 1_555 . 1_555 n
O1 Ge O3 111.42(13) 1_555 . -4_556 n
O1 Ge O5 89.1(13) 1_555 . 6_554 n
O1 Ge O5 89.1(13) 1_555 . -3_556 n
O2 Ge O3 106.04(15) 1_555 . 1_555 n
O2 Ge O3 106.04(15) 1_555 . -4_556 n
O2 Ge O5 138.7(12) 1_555 . 6_554 n
O2 Ge O5 138.7(12) 1_555 . -3_556 n
O3 Ge O3 104.72(19) 1_555 . -4_556 n
O3 Ge O5 32.7(12) 1_555 . 6_554 n
O3 Ge O5 92.3(10) 1_555 . -3_556 n
O3 Ge O5 92.3(10) -4_556 . 6_554 n
O3 Ge O5 32.7(12) -4_556 . -3_556 n
O5 Ge O5 67.6(20) 6_554 . -3_556 n
La1 O1 La2 107.44(10) 3_555 . 1_555 n
La1 O1 La2 107.46(10) 3_555 . -2_566 n
La1 O1 Ge 95.55(16) 3_555 . 1_555 n
La2 O1 La2 93.36(14) 1_555 . -2_566 n
La2 O1 Ge 125.83(10) 1_555 . 1_555 n
La2 O1 Ge 125.81(10) -2_566 . 1_555 n
La1 O2 La2 116.74(9) 5_665 . 2_655 n
La1 O2 La2 116.74(9) 5_665 . -1_665 n
La1 O2 Ge 120.76(19) 5_665 . 1_555 n
La2 O2 La2 91.92(14) 2_655 . -1_665 n
La2 O2 Ge 103.01(11) 2_655 . 1_555 n
La2 O2 Ge 103.03(11) -1_665 . 1_555 n
La1 O3 La1 116.32(13) 1_555 . 2_554 n
La1 O3 Ge 96.29(11) 1_555 . 1_555 n
La1 O3 O5 73.5(21) 1_555 . 6_554 n
La1 O3 Ge 140.28(15) 2_554 . 1_555 n
La1 O3 O5 86.1(18) 2_554 . 6_554 n
Ge O3 O5 81.9(17) 1_555 . 6_554 n
La1 O4 La1 120.0 1_555 . 3_555 n
La1 O4 La1 120.0 1_555 . 5_555 n
La1 O4 La1 120.0 3_555 . 5_555 n
La1 O5 La1 114.6(13) 2_555 . 3_555 n
La1 O5 La1 105.9(13) 2_555 . 4_555 n
La1 O5 Ge 95.6(15) 2_555 . 2_555 n
La1 O5 O3 83.7(25) 2_555 . 2_555 n
La1 O5 La1 115.9(16) 3_555 . 4_555 n
La1 O5 Ge 122.4(17) 3_555 . 2_555 n
La1 O5 O3 70.4(16) 3_555 . 2_555 n
La1 O5 Ge 99.5(14) 4_555 . 2_555 n
La1 O5 O3 163.2(26) 4_555 . 2_555 n
Ge O5 O3 65.4(19) 2_555 . 2_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1 4.0645(29) . 3_555 n
La1 La1 4.0645(29) . 5_555 n
La1 Ge 3.3359(33) . 1_555 n
La1 Ge 3.4025(31) . 5_555 n
La1 O1 2.763(5) . 5_555 n
La1 O2 2.5834(31) . 3_655 n
La1 O3 2.6580(32) . 1_555 n
La1 O3 2.4540(22) . 6_555 n
La1 O3 2.4540(22) . -3_555 n
La1 O3 2.6580(32) . -4_556 n
La1 O4 2.3466(17) . 1_555 n
La1 O5 2.53(4) . 4_554 n
La1 O5 2.599(29) . 5_555 n
La1 O5 2.56(4) . 6_554 n
La1 O5 2.53(4) . -1_556 n
La1 O5 2.599(29) . -2_556 n
La1 O5 2.56(4) . -3_556 n
La2 La2 3.705(6) . -2_565 n
La2 La2 3.607(6) . -2_566 n
La2 Ge 3.4204(22) . 2_554 n
La2 Ge 3.4209(22) . 4_664 n
La2 Ge 3.4200(22) . 6_564 n
La2 O1 2.4789(32) . 1_555 n
La2 O1 2.4786(32) . 3_665 n
La2 O1 2.4782(32) . 5_565 n
La2 O2 2.5766(32) . 2_554 n
La2 O2 2.5772(32) . 4_664 n
La2 O2 2.5767(32) . 6_564 n
La2 O3 2.941(4) . -1_665 n
La2 O3 2.940(4) . -3_565 n
La2 O3 2.940(4) . -5_555 n
Ge La1 3.3359(33) . 1_555 n
Ge La1 3.4025(31) . 3_555 n
Ge La2 3.4200(22) . 2_655 n
Ge La2 3.4209(22) . -1_665 n
Ge O1 1.7365(32) . 1_555 n
Ge O2 1.7424(30) . 1_555 n
Ge O3 1.7456(24) . 1_555 n
Ge O3 1.7456(24) . -4_556 n
Ge O5 1.900(34) . 6_554 n
Ge O5 1.900(34) . -3_556 n
O1 La1 2.763(5) . 3_555 n
O1 La2 2.4789(32) . 1_555 n
O1 La2 2.4786(32) . -2_566 n
O1 Ge 1.7365(32) . 1_555 n
O2 La1 2.5834(31) . 5_665 n
O2 La2 2.5767(32) . 2_655 n
O2 La2 2.5772(32) . -1_665 n
O2 Ge 1.7424(30) . 1_555 n
O3 La1 2.6580(32) . 1_555 n
O3 La1 2.4540(22) . 2_554 n
O3 La2 2.941(4) . -1_665 n
O3 Ge 1.7456(24) . 1_555 n
O3 O5 1.04(4) . 6_554 n
O4 La1 2.3466(17) . 1_555 n
O4 La1 2.3466(17) . 3_555 n
O4 La1 2.3466(17) . 5_555 n
O5 La1 2.56(4) . 2_555 n
O5 La1 2.599(29) . 3_555 n
O5 La1 2.53(4) . 4_555 n
O5 Ge 1.900(34) . 2_555 n
O5 O3 1.04(4) . 2_555 n
O5 O5 2.12(6) . -4_557 n
loop_
_pd_phase_block_id
2003-09-18T17:07|La960Ge_773k_phase1|La960Ge_773K||
2003-09-18T17:07|La960Ge_773k_phase2|La960Ge_773K||
2003-09-18T17:07|La960Ge_773k_phase3|La960Ge_773K||
